Search

Collections

Journals

About

Contact us

My IOPscience

Trends in magnetism of free Rh clusters via relativistic ab-initio calculations

This content has been downloaded from IOPscience. Please scroll down to see the full text. 2015 J. Phys.: Condens. Matter 27 056004 (http://iopscience.iop.org/0953-8984/27/5/056004) View the table of contents for this issue, or go to the journal homepage for more

Download details: IP Address: 137.149.200.5 This content was downloaded on 21/02/2015 at 06:07

Please note that terms and conditions apply.

Journal of Physics: Condensed Matter J. Phys.: Condens. Matter 27 (2015) 056004 (8pp)

doi:10.1088/0953-8984/27/5/056004

Trends in magnetism of free Rh clusters via relativistic ab-initio calculations ˇ 1,4 , H Ebert2 and J Minar ´ 2,3 O Sipr 1

Institute of Physics of the ASCR v. v. i., Cukrovarnick´a 10, CZ-162 53 Prague, Czech Republic Department Chemie, Universit¨at M¨unchen, Butenandtstr. 5-13, D-81377 M¨unchen, Germany 3 New Technologies Research Centre, University of West Bohemia, Univerzitn´ı 2732, 306 14 Pilsen, Czech Republic 2

E-mail: [email protected] Received 7 November 2014, revised 3 December 2014 Accepted for publication 10 December 2014 Published 21 January 2015 Abstract

A fully relativistic ab-initio study on free Rh clusters of 13–135 atoms is performed to identify general trends concerning their magnetism and to check whether concepts which proved to be useful in interpreting magnetism of 3d metals are applicable to magnetism of 4d systems. We found that there is no systematic relation between local magnetic moments and coordination numbers. On the other hand, the Stoner model appears well-suited both as a criterion for the onset of magnetism and as a guide for the dependence of local magnetic moments on the site-resolved density of states at the Fermi level. Large orbital magnetic moments antiparallel to spin magnetic moments were found for some sites. The intra-atomic magnetic dipole Tz term can be quite large at certain sites but as a whole it is unlikely to affect the interpretation of x-ray magnetic circular dichroism experiments based on the sum rules. Keywords: clusters, magnetism, Stoner criterion, anisotropy (Some figures may appear in colour only in the online journal)

monotonous way and become strongly suppressed (possibly to zero) for clusters of more than 60 atoms. Another experimental input comes from x-ray magnetic circular dichroism (XMCD) measurements of Sessi et al [2] who studied quasi-free Rh clusters of few tens of atoms in a Xe matrix on Ag(1 0 0) and found that the clusters are magnetic, with an effective spin magnetic moment µspin of about 0.26 µB and with the ratio between orbital and spin magnetic moments µorb /µspin about 40%. Recently, spin and orbital moments induced in paramagnetic Rh clusters of about 220 atoms embedded in a Al2 O3 matrix were determined also via XMCD [3] and it was found that the orbital moment µorb does not exceed 2% of µspin . For a deeper understanding of the magnetism of free Rh clusters and of Rh magnetism in general it would be useful to identify general trends which Rh-based systems obey. This could be achieved by monitoring the trends for a large set of related systems and comparing them with the situation for (much better studied) 3d elements. Such a study should be performed in a relativistic way because only then possible effects of SOC can be properly included. Also, experiments pose some questions that call for fully relativistic calculations—such as the above mentioned issue of small

1. Introduction

Magnetism of systems with reduced dimensions is a vivid research area both because of fundamental interest and because of technological relevance. To be able to design new devices based on magnetism of clusters and thin films one should have an intuitive understanding for these, so that one can estimate beforehand which configurations and compositions might be perspective or not. Magnetism of Rh carries a special appeal because it concerns a material which is magnetic only in reduced dimensions and in which the spin orbit coupling (SOC) is expected to play a more important role than in the magnetism of 3d elements. Indeed, Rh magnetism seems to be quite intriguing, with results obtained so far being often controversial and not easy to interpret. Catalytic properties of Rh add yet another impetus for studying low-dimensional Rh systems. The interest in free Rh clusters was stimulated by a Stern– Gerlach-type experiment on clusters of 9–100 atoms [1], where it was found that Rh clusters have magnetic moments which decrease with cluster size down from 0.8 µB in a non4

www.fzu.cz/∼sipr.

0953-8984/15/056004+08$33.00

1

© 2015 IOP Publishing Ltd Printed in the UK

ˇ O Sipr et al

J. Phys.: Condens. Matter 27 (2015) 056004

µorb measured by XMCD for a set of paramagnetic clusters embedded in Als O3 [3] in contrast to large µorb measured for ferromagnetic clusters in a Xe matrix [2]. A considerable effort was devoted to theoretical research on free Rh clusters recently. Even though interesting and important results were obtained, only few systematic studies for large sets of systems were done so only an incomplete picture could have been gathered. This is even more true concerning relativistic properties such as orbital magnetism. Most ab initio studies focused on clusters of less than 20 atoms and specifically on their geometries. It turns out that small clusters often tend to have non-compact shapes [4–6]. The situation is still not clear because different density functional theory (DFT) implementations predict different structures and spin configurations [7]. Pseudopotential calculations seem to give rise to more open structures than all-electron calculations [8]. Structural studies for large clusters were performed only within a model d-band tight-binding (TB) Hamiltonian and it was found that the relaxation of bond distances for fcc clusters of 13–165 atoms is non-uniform, with some distances decreasing and some distances increasing [9]. It emerges that the existence of more competing configurations is typical for Rh clusters and sometimes the configurations differ only little in energies but considerably in magnetic moments [10–13]. It seems that a similar situation arises regarding the suppression of magnetism for large clusters, which occurs for sizes between 60 and 100 atoms according to the experiment [1]. E.g. model Hamiltonian calculations found that for fcc clusters of 55 and 79 atoms magnetic solutions exist but are higher in energy than nonmagnetic solutions [9]. For clusters of 135 and 165 atoms, no magnetic solutions were found [9]. Pseudopotential calculations for icosahedral clusters yield a finite moment for a 55 atoms cluster and a zero moment for a 147 atoms cluster [12]. At the same time, in order to explain their XMCD experiments, Barthem et al [3] suggest that the Stoner criterion may be locally fulfilled at only some atoms in large Rh clusters, giving rise to an inhomogeneous magnetic state. Connected with the question of size-dependence of magnetic moments is the question of the dependence of local magnetic moments on the coordination numbers. For 3d clusters (both free [14] and supported) [15–17] a distinct relation could be identified in this respect. However, this need not be transferable to 4d clusters and there are some hints that a relation of this kind may be absent in Rh systems [4, 6, 18]. However, no systematic study about this has been performed so far. The issue of orbital moments has not yet attracted much theoretical attention. Model d-band TB Hamiltonian calculations were performed for few Rh clusters of up to 27 atoms [19, 20]. It was found that µorb is typically 10–20% of µspin . The orbital moment µorb is nearly always parallel to µspin and when it is antiparallel to µspin , it is very small. Ab initio calculations performed for Rh clusters of 2–7 atoms lead to similar conclusions: spin and orbital magnetic moments are always parallel to each other and the µorb /µspin ratio is about 10%, except for the smallest clusters [21]. In all these studies the SOC was added in a second variation approach.

However, the SOC may play a more important role in 4d clusters and it is not clear whether it can be fully accounted for in this way. Recalling also that recent XMCD studies led to opposite conclusions regarding the µorb /µspin ratio [2, 3], a more detailed study of orbital magnetism of Rh clusters is desirable. Concerning the interpretation of experiments, let us mention finally that the XMCD sum rules do not provide a ‘bare’ spin moment µspin but only its combination with the magnetic dipole Tz term, µspin + 7Tz . It is conceivable that a disagreement between theory and experiment may arise partly due to the effect of the Tz term [3]. Earlier calculations for Rh19 and Rh43 clusters suggest that this influence should not be crucial for free clusters [2] but this ought to be analyzed more deeply and for a large set of systems. It turns out that despite the intense attention that has been devoted to theoretical research on free Rh clusters, some important issues remain to be solved. One of them is whether there is any systematic relation between local magnetic moments and coordination numbers as in 3d clusters or whether such a relation is totally absent. Linked to this is a question whether the Stoner criterion can be applied locally, i.e. whether it could be used to estimate local magnetic moments in large clusters. The relatively large SOC implies a question to what extent will scalar-relativistic results differ from fullyrelativistic results. How important is orbital magnetism in Rh clusters, especially in large ones? Is it possible to reconcile large µorb /µspin ratios obtained via XMCD by Sessi et al [2] with small µorb /µspin ratios obtained by Barthem et al [3]? What is the role of the magnetic dipole term Tz ? Could it possibly be responsible for the deviations between some theories and XMCD experiments? To address these issues, we performed a fully-relativistic theoretical study of clusters of 13–135 atoms and also of free-standing monolayers (for comparison). We found that some important intuitive concepts which proved to be useful in magnetism of 3d metals, such as the relationship between magnetic moments and coordination numbers, are not applicable to Rh clusters (and surfaces alike). Some other concepts, such as the Stoner model linking magnetic moments to DOS at the Fermi level, remain to be valid and useful. 2. Computational method

The calculations were performed in an ab-initio way within the spin density functional theory, relying on the local spin density approximation (LSDA) as parametrized by Vosko et al [22]. The electronic structure is described fully relativistically by the corresponding Dirac equation. The computational approach is based on the multiple-scattering or Korringa–Kohn–Rostoker formalism [23] as implemented in the SPRKKR code [24]. The electronic structure problem is solved completely in real space. The potentials were treated within the atomic sphere approximation (ASA). For the angular momentum expansion of the Green function, a cutoff of max = 3 was used. Only collinear magnetic structures were considered in this study. The clusters were assumed to be spherical-like, containing 13–135 atoms, with fcc geometry as if cut from the bulk Rh 2

ˇ O Sipr et al

J. Phys.: Condens. Matter 27 (2015) 056004

Table 1. Local magnetic moments for clusters of different sizes, resolved according to the distance R from the cluster center. Each cluster is represented by one column.

R 0.00

Rh13 1.068 −0.013 −0.012

1.90

2.69

3.29

3.80

Rh14

Rh19

Rh38

0.484 −0.170 −0.352 1.193 0.032 0.027

1.452 0.118 0.081

Rh43

Rh55

−0.007 −0.047 n/a

0.011 0.029 n/a

0.457 −0.046 −0.101 0.864 0.138 0.161

1.306 0.234 0.179

0.01 0.01 n/a 0.099 −0.011 −0.108

0.296 −0.013 −0.044

0.680 −0.028 −0.041 0.632 0.100 0.160

0.008 0.000 n/a 0.495 0.028 0.056

4.25

0.847 0.050 0.059

0.761 0.085 0.112

4.65

0.004 0.003 n/a 0.190 0.017 0.087

5.38

5.71

Rh68

0.718 0.060 0.084 0.254 0.035 0.139 0.134 0.016 0.062

Note: The first line for each R stands for µspin , the second for µorb and the third for the ratio µorb /µspin (shown only if µspin is larger than 0.05 µB ). The unit for R is Å, the unit for µspin and µorb is µB .

crystal. They are centered either around an atom (13, 19, 43, 55, 79, 87, and 135 atoms) or around an interstitial empty site (14, 38, and 68 atoms). No structural relaxation was performed. The vacuum region was represented by empty sites located at lattice points. The network of these empty sites was built so that an empty site was included if it was a first- or second-nearest neighbor to any cluster atom. We also performed some comparative calculations for isolated or free-standing (0 0 1), (1 1 0), and (1 1 1) monolayers and for the (0 0 1) crystal surface. These calculations were performed using supercell (multilayer) geometries. To simulate the crystal surface, we employed a slab consisting of 17 layers of Rh atoms. Successive Rh monolayers or slabs were separated by 13–20 Å of vacuum in the supercell. The integration over the k-points was done on a regular mesh and for each of the systems the integration grid was chosen so that its density corresponds to (at least) 15 625 k-points in the full Brillouin zone of the bulk Rh crystal. Otherwise the calculations were done as for the free clusters.

the same coordination shell need not be symmetry equivalent. Each value in table 1 thus represents an average over all atoms located at the same distance R from the center of the cluster. The magnetization M is parallel to the (0 0 1) direction of the parental fcc lattice. No stable magnetic state was found for the 79 atoms and 87 atoms clusters. For the 135 atoms cluster a metastable magnetic state was identified (see also section 3.3 below), with sizable magnetic moments only at the last two coordination spheres: the average µspin (µorb ) at the distance of 6.59 Å is 0.091 µB (0.017 µB ) and average µspin (µorb ) at the distance of 7.12 Å is 0.271 µB (0.025 µB ). Concerning the angular-momentum decomposition, the d component of µspin comprises 90–95% of its total value. For µorb the dominance of the d component is even more pronounced. A better idea how the magnetic profiles look like may be obtained from representative graphs in figure 1. It appears from all the data that there is hardly any common trend in these profiles. This is in contrast to the case of 3d clusters where µspin and µorb generally increase towards the surface for all cluster sizes [14].

3. Results 3.1. Magnetic moments

3.2. Relation between local µspin and the coordination number

Local moments µspin , µorb and the ratio µorb /µspin for clusters of 13–68 atoms are shown in table 1. Note that because of the presence of magnetization and of the SOC, atoms belonging to

Our study covers a wide range of cluster sizes so it is possible to perform a systematic search for a relation between local 3

ˇ O Sipr et al

J. Phys.: Condens. Matter 27 (2015) 056004 1.0

0.2 0.1

[ 0.4

19 38 55

orb

spin

19 38 55

0.0 0.0

-0.1

orb/ spin

B]

0.6

[

B]

0.8

19 38 55

-0.2

0.2

spin

orb/ spin

orb

0.0

-0.2 0

1

2

3

4

5

distance from center

˚ [A]

-0.4 0

1

2

3

4

5

distance from center

˚ [A]

0

4

5

distance from center

1

2

3

˚ [A]

Figure 1. Magnetic profiles for clusters of 19, 38, and 55 atoms. Left and middle panels show µspin and µorb averaged over all atoms at given distance from the center. The right panel shows corresponding ratios of µorb and µspin (the data point at R = 0 for the 55 atoms cluster was omitted because the corresponding µspin is very small). Table 2. Average magnetic moments in µB and magnetization energies per atom in mRy for clusters of 13–135 atoms. Apart from fully-relativistic results we display also µspin and Emag obtained via scalar-relativistic calculations.

13 14 19 38 43 55 68 135

1.0

spin

[

B]

1.5

0.5

0.0 4

6

8

10

N

µspin

µspin scalar

µorb

Emag

Emag scalar

13 14 19 38 43 55 68 135

1.423 1.258 0.771 0.696 0.202 0.526 0.062 0.107

1.604 1.433 0.823 0.785 0.254 0.563 0.088 0.216

0.108 0.147 0.110 0.040 0.009 0.037 0.009 0.007

−11.74 −2.88 −2.34 −0.61 −0.15 −0.66 0.00 0.01

−13.82 −3.55 −2.63 −1.47 −0.22 −1.15 −0.06 0.12

12

number of nearest neighbors

monotonously. For the 68 atoms cluster the magnetic and non-magnetic states are practically degenerate, whereas for the 135 atoms cluster the ground state is non-magnetic. For a better understanding of the Emag values, recall that corresponding values for bulk 3d metals are 31.2 mRy, 29.8 mRy, and 3.6 mRy for Fe, Co, and Ni, respectively. Our results indicate that for large Rh clusters metastable isomers with different magnetic configurations should be expected, similarly as it was found for small Rh clusters [10–13]. One can see from table 2 that the scalar-relativistic approximation overestimates µspin typically by about 10% (except for large clusters and/or small µspin where the relative difference is larger). In line with this, scalar-relativistic calculations yield larger magnetization energies.

Figure 2. Local µspin as a function of the coordination number for

atoms in clusters of 13–135 atoms.

moments and coordination numbers. Earlier studies failed to find a common trend like the one which had been identified before for the 3d clusters but in those studies always only a small range of cluster sizes was explored [4, 6, 18]. We display in figure 2 local µspin as a function of the coordination number for magnetic clusters containing up to 135 atoms (including thus also the metastable 135 atoms cluster). It is evident from our data that no common rule concerning all atoms can be drawn for free Rh clusters. 3.3. Average magnetic moments and magnetization energies

3.4. Stoner criterion applied locally

A simple estimate of the strength of the magnetization can be obtained from average magnetic moments and from magnetization energies (differences of total energies per atom for a magnetic and a non-magnetic state). Furthermore, these quantities can be evaluated using fully-relativistic calculations and using the scalar-relativistic approximation [25], providing thus an idea on the role of the SOC. We summarized these results in table 2. Note that µorb is zero in the scalar-relativistic approximation. Average magnetic moments as well as magnetization energies generally decrease with cluster size, albeit non-

When debating about magnetism of elements such as Ru, Rh, Pd, it is often argued that these metals could become magnetic in lower dimensions because then their density of states (DOS) at the Fermi energy n(EF ) might increase due to band-narrowing, meaning that the Stoner criterion Is n(EF ) > 1 ,

(1)

with Is being the Stoner integral, would be satisfied. It would be interesting to see to what extent does this criterion really 4

ˇ O Sipr et al

J. Phys.: Condens. Matter 27 (2015) 056004

n(EF ) for every atom in all the clusters we investigate. If we choose ImE = 3 mRy, we obtain a graph for the dependence of the local µspin on the corresponding n(EF ) shown in figure 3. The thick vertical gray line in figure 3 highlights the ‘critical DOS’ which separates magnetic systems from non-magnetic systems according to equation (1). One can see that the Stoner criterion (1) can be used with a good accuracy to predict whether a particular Rh atom will be magnetic or not. To be more precise, it follows from figure 3 that the criterion (1) is a bit too strict—one can get magnetism also for atoms where n(EF ) is by 10–20% lower than the critical value. If the Stoner model for the dependence of µspin on n(EF ) is adopted, [30] 1 1 , ⇔ n(EF ) > µspin ∼ 1 − Is n(EF ) Is

Table 3. Stoner exchange integral Is , DOS per spin channel at EF in a non-magnetic state, Stoner product Is n(EF ) and magnetic moment for 2D Rh systems.

System

(1 0 0) Monolayer (1 1 0) Monolayer (1 1 1) Monolayer (1 0 0) Surface Bulk

Is

n(EF )

mRy

Ry−1

46.7 45.5 45.2 44.9 48.2

18.0 18.5 24.3 11.4 9.9

Is n(EF )

µspin µB

0.84 0.84 1.10 0.51 0.48

0.00 0.00 0.40 0.00 0.00

µspin = 0

⇔

n(EF )